#------------------------------------------------------------------------------
#$Date: 2016-10-29 08:28:54 +0200 (Sat 29 de Oct de 2016) $
#$Revision: 187682 $
#$URL: svn://www.crystallography.net/cod/cif/7/22/69/7226963.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_7226963
loop_
_publ_author_name
'Sha, JingQuan'
'Yang, Xi-Ya'
'Zhu, Pei-Pei'
'Lan, Ya-Qian'
'Sheng, Ning'
_publ_section_title
;
 Two new silver triazole frameworks with polyoxometalate templates
;
_journal_name_full               'RSC Adv.'
_journal_paper_doi               10.1039/C6RA23809B
_journal_year                    2016
_chemical_formula_moiety         'C12 H12 Ag5 Mo12 N18 O40 P'
_chemical_formula_sum            'C12 H12 Ag5 Mo12 N18 O40 P'
_chemical_formula_weight         2770.00
_space_group_crystal_system      trigonal
_space_group_IT_number           162
_space_group_name_Hall           '-P 3 2'
_space_group_name_H-M_alt        'P -3 1 m'
_symmetry_space_group_name_Hall  '-P 3 2'
_symmetry_space_group_name_H-M   'P -3 1 m'
_atom_sites_solution_hydrogens   geom
_audit_creation_method           SHELXL-2014/7
_audit_update_record
;
2016-07-20 deposited with the CCDC.
2016-10-28 downloaded from the CCDC.
;
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            1
_cell_length_a                   12.1615(3)
_cell_length_b                   12.1615(3)
_cell_length_c                   10.4558(5)
_cell_measurement_reflns_used    10628
_cell_measurement_temperature    273(2)
_cell_measurement_theta_max      29.282
_cell_measurement_theta_min      3.350
_cell_volume                     1339.25(8)
_computing_cell_refinement       'Bruker FRAMBO'
_computing_data_collection       'Bruker FRAMBO'
_computing_data_reduction        'Bruker SHELXTL'
_computing_molecular_graphics    'Bruker SHELXTL'
_computing_publication_material  'Bruker SHELXTL'
_computing_structure_refinement  'SHELXL-2014/7 (Sheldrick, 2014)'
_computing_structure_solution    'Bruker SHELXTL'
_diffrn_ambient_temperature      273(2)
_diffrn_measured_fraction_theta_full 0.997
_diffrn_measured_fraction_theta_max 0.952
_diffrn_measurement_device_type  'multiwire proportional'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0410
_diffrn_reflns_av_unetI/netI     0.0265
_diffrn_reflns_Laue_measured_fraction_full 0.997
_diffrn_reflns_Laue_measured_fraction_max 0.952
_diffrn_reflns_limit_h_max       16
_diffrn_reflns_limit_h_min       -16
_diffrn_reflns_limit_k_max       15
_diffrn_reflns_limit_k_min       -16
_diffrn_reflns_limit_l_max       14
_diffrn_reflns_limit_l_min       -11
_diffrn_reflns_number            10628
_diffrn_reflns_point_group_measured_fraction_full 0.997
_diffrn_reflns_point_group_measured_fraction_max 0.952
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         29.282
_diffrn_reflns_theta_min         3.350
_exptl_absorpt_coefficient_mu    4.630
_exptl_crystal_colour            yellow
_exptl_crystal_density_diffrn    3.435
_exptl_crystal_description       block
_exptl_crystal_F_000             1284
_refine_diff_density_max         1.085
_refine_diff_density_min         -1.275
_refine_diff_density_rms         0.181
_refine_ls_extinction_coef       0.0014(3)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_extinction_method     'SHELXL-2014/7 (Sheldrick 2014'
_refine_ls_goodness_of_fit_ref   1.036
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     109
_refine_ls_number_reflns         1262
_refine_ls_number_restraints     123
_refine_ls_restrained_S_all      1.055
_refine_ls_R_factor_all          0.0670
_refine_ls_R_factor_gt           0.0534
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[σ²(Fo²)+(0.0432P)²+24.0000P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1224
_refine_ls_wR_factor_ref         0.1291
_reflns_Friedel_coverage         0.000
_reflns_number_gt                1053
_reflns_number_total             1262
_reflns_threshold_expression     'I > 2σ(I)'
_cod_data_source_file            c6ra23809b2.cif
_cod_data_source_block           shelx
_cod_original_cell_volume        1339.25(11)
_cod_database_code               7226963
_shelx_shelxl_version_number     2014/7
_shelx_space_group_comment
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
loop_
_space_group_symop_operation_xyz
'x, y, z'
'-y, x-y, z'
'-x+y, -x, z'
'-y, -x, -z'
'x, x-y, -z'
'-x+y, y, -z'
'-x, -y, -z'
'y, -x+y, -z'
'x-y, x, -z'
'y, x, z'
'-x, -x+y, z'
'x-y, -y, z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
Mo1 Mo 0.83216(8) 0.83216(8) 0.27671(9) 0.0326(3) Uani 1 2 d S TU P . .
Mo2 Mo 0.66409(9) 0.83205(4) 0.0000 0.0312(3) Uani 1 2 d S TU P . .
P1 P 1.0000 1.0000 0.0000 0.0160(11) Uani 1 12 d S TU P . .
O4 O 0.5077(8) 0.7538(4) 0.0000 0.047(2) Uani 1 2 d S TU P . .
O2 O 0.7525(8) 0.7525(8) 0.4045(8) 0.053(2) Uani 1 2 d S TU P . .
O3 O 0.6976(8) 0.8213(8) 0.1755(6) 0.061(2) Uani 1 1 d . U . . .
O9 O 0.7004(10) 1.0000 0.0295(9) 0.058(3) Uani 1 2 d S TU P . .
O1 O 1.0000 0.8746(8) 0.3184(12) 0.059(3) Uani 1 2 d S TU P . .
O6 O 0.8816(11) 0.8816(11) 0.0483(13) 0.023(2) Uani 0.5 2 d S TU P . .
O5 O 1.0000 1.0000 -0.145(2) 0.021(4) Uani 0.5 6 d S TU P . .
Ag1 Ag 0.3333 0.6667 0.7815(3) 0.0529(7) Uani 0.5 3 d S TU P . .
Ag2 Ag 0.77660(12) 0.5532(2) 0.5000 0.0538(6) Uani 0.5 2 d S TU P . .
N1 N 0.4578(19) 0.586(2) 0.7242(19) 0.043(4) Uani 0.5 1 d . U P A -1
N2 N 0.578(2) 0.498(2) 0.729(2) 0.047(5) Uani 0.5 1 d . U P A -1
N3 N 0.6208(17) 0.5810(17) 0.6296(16) 0.048(4) Uani 0.5 1 d . U P A -1
C1 C 0.4835(16) 0.5050(18) 0.7828(17) 0.044(4) Uani 0.5 1 d . U P A -1
H1 H 0.4396 0.4579 0.8543 0.053 Uiso 0.5 1 calc R U P A -1
C2 C 0.5426(19) 0.640(2) 0.6300(19) 0.040(4) Uani 0.5 1 d . U P A -1
H2 H 0.5500 0.7034 0.5751 0.047 Uiso 0.5 1 calc R U P A -1
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ag Ag -0.8971 1.1015 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Mo Mo -1.6832 0.6857 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
P P 0.1023 0.0942 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
O2 Mo1 O1 102.2(4) . .
O2 Mo1 O1 102.2(4) . 3_675
O1 Mo1 O1 88.7(6) . 3_675
O2 Mo1 O3 100.3(4) . .
O1 Mo1 O3 157.5(5) . .
O1 Mo1 O3 87.9(4) 3_675 .
O2 Mo1 O3 100.3(4) . 10
O1 Mo1 O3 87.9(4) . 10
O1 Mo1 O3 157.5(5) 3_675 10
O3 Mo1 O3 86.7(4) . 10
O2 Mo1 O6 158.2(5) . .
O1 Mo1 O6 93.4(4) . .
O1 Mo1 O6 93.4(4) 3_675 .
O3 Mo1 O6 64.7(3) . .
O3 Mo1 O6 64.7(3) 10 .
O2 Mo1 O5 160.0(6) . 7_775
O1 Mo1 O5 64.4(4) . 7_775
O1 Mo1 O5 64.4(4) 3_675 7_775
O3 Mo1 O5 94.2(4) . 7_775
O3 Mo1 O5 94.2(4) 10 7_775
O6 Mo1 O5 41.8(5) . 7_775
O4 Mo2 O9 101.7(4) . 9_655
O4 Mo2 O9 101.7(4) . .
O9 Mo2 O9 156.6(7) 9_655 .
O4 Mo2 O3 100.7(3) . .
O9 Mo2 O3 87.1(3) 9_655 .
O9 Mo2 O3 88.5(4) . .
O4 Mo2 O3 100.7(3) . 5_565
O9 Mo2 O3 88.5(4) 9_655 5_565
O9 Mo2 O3 87.1(3) . 5_565
O3 Mo2 O3 158.5(5) . 5_565
O4 Mo2 O6 159.0(3) . .
O9 Mo2 O6 64.0(4) 9_655 .
O9 Mo2 O6 93.5(4) . .
O3 Mo2 O6 64.9(4) . .
O3 Mo2 O6 94.4(4) 5_565 .
O4 Mo2 O6 159.0(3) . 8_565
O9 Mo2 O6 93.5(4) 9_655 8_565
O9 Mo2 O6 64.0(4) . 8_565
O3 Mo2 O6 94.4(4) . 8_565
O3 Mo2 O6 64.9(4) 5_565 8_565
O6 Mo2 O6 42.0(6) . 8_565
O5 P1 O5 180.0 7_775 .
O5 P1 O6 109.3(5) 7_775 9_655
O5 P1 O6 70.7(5) . 9_655
O5 P1 O6 109.3(5) 7_775 7_775
O5 P1 O6 70.7(5) . 7_775
O6 P1 O6 109.6(5) 9_655 7_775
O5 P1 O6 70.7(5) 7_775 2_765
O5 P1 O6 109.3(5) . 2_765
O6 P1 O6 70.4(5) 9_655 2_765
O6 P1 O6 70.4(5) 7_775 2_765
O5 P1 O6 109.3(5) 7_775 8_565
O5 P1 O6 70.7(5) . 8_565
O6 P1 O6 109.6(5) 9_655 8_565
O6 P1 O6 109.6(5) 7_775 8_565
O6 P1 O6 180.0 2_765 8_565
O5 P1 O6 70.7(5) 7_775 3_675
O5 P1 O6 109.3(5) . 3_675
O6 P1 O6 180.0(10) 9_655 3_675
O6 P1 O6 70.4(5) 7_775 3_675
O6 P1 O6 109.6(5) 2_765 3_675
O6 P1 O6 70.4(5) 8_565 3_675
O5 P1 O6 70.7(5) 7_775 .
O5 P1 O6 109.3(5) . .
O6 P1 O6 70.4(5) 9_655 .
O6 P1 O6 180.0 7_775 .
O6 P1 O6 109.6(5) 2_765 .
O6 P1 O6 70.4(5) 8_565 .
O6 P1 O6 109.6(5) 3_675 .
Mo1 O3 Mo2 137.9(4) . .
Mo2 O9 Mo2 139.3(6) . 8_565
Mo1 O1 Mo1 138.7(6) 2_765 .
P1 O6 O5 54.4(7) . 7_775
P1 O6 O6 54.8(3) . 9_655
O5 O6 O6 89.7(6) 7_775 9_655
P1 O6 O6 54.8(3) . 8_565
O5 O6 O6 89.7(6) 7_775 8_565
O6 O6 O6 90.3(11) 9_655 8_565
P1 O6 Mo2 123.8(4) . 9_655
O5 O6 Mo2 131.3(3) 7_775 9_655
O6 O6 Mo2 69.0(3) 9_655 9_655
O6 O6 Mo2 131.6(10) 8_565 9_655
P1 O6 Mo2 123.8(4) . .
O5 O6 Mo2 131.3(3) 7_775 .
O6 O6 Mo2 131.6(10) 9_655 .
O6 O6 Mo2 69.0(3) 8_565 .
Mo2 O6 Mo2 92.3(5) 9_655 .
P1 O6 Mo1 123.5(7) . .
O5 O6 Mo1 69.1(7) 7_775 .
O6 O6 Mo1 131.1(8) 9_655 .
O6 O6 Mo1 131.1(8) 8_565 .
Mo2 O6 Mo1 92.2(4) 9_655 .
Mo2 O6 Mo1 92.2(4) . .
P1 O5 O6 55.0(7) . 7_775
P1 O5 O6 55.0(7) . 9_655
O6 O5 O6 90.3(10) 7_775 9_655
P1 O5 O6 55.0(7) . 8_565
O6 O5 O6 90.3(10) 7_775 8_565
O6 O5 O6 90.3(10) 9_655 8_565
P1 O5 Mo1 124.0(4) . 8_565
O6 O5 Mo1 131.34(13) 7_775 8_565
O6 O5 Mo1 131.34(13) 9_655 8_565
O6 O5 Mo1 69.1(5) 8_565 8_565
P1 O5 Mo1 124.0(4) . 9_655
O6 O5 Mo1 131.34(13) 7_775 9_655
O6 O5 Mo1 69.1(5) 9_655 9_655
O6 O5 Mo1 131.34(13) 8_565 9_655
Mo1 O5 Mo1 91.7(6) 8_565 9_655
P1 O5 Mo1 124.0(4) . 7_775
O6 O5 Mo1 69.1(5) 7_775 7_775
O6 O5 Mo1 131.34(13) 9_655 7_775
O6 O5 Mo1 131.34(13) 8_565 7_775
Mo1 O5 Mo1 91.7(6) 8_565 7_775
Mo1 O5 Mo1 91.7(6) 9_655 7_775
N1 Ag1 N2 117.5(8) . 11_665
N3 Ag2 N3 166.5(8) 6_656 .
C1 N1 C2 107.3(18) . .
C1 N1 Ag1 131.3(15) . .
C2 N1 Ag1 119.9(14) . .
C1 N2 N3 107.4(17) . .
C1 N2 Ag1 128.9(13) . 12_665
N3 N2 Ag1 123.4(14) . 12_665
N2 N3 C2 105.4(18) . .
N2 N3 Ag2 110.4(13) . .
C2 N3 Ag2 143.3(14) . .
N1 C1 N2 112.7(17) . .
N1 C1 H1 123.6 . .
N2 C1 H1 123.6 . .
N1 C2 N3 107.0(18) . .
N1 C2 H2 126.5 . .
N3 C2 H2 126.5 . .
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
Mo1 O2 1.650(8) .
Mo1 O1 1.889(4) .
Mo1 O1 1.889(4) 3_675
Mo1 O3 1.897(7) .
Mo1 O3 1.897(7) 10
Mo1 O6 2.462(13) .
Mo1 O5 2.463(13) 7_775
Mo2 O4 1.647(8) .
Mo2 O9 1.887(4) 9_655
Mo2 O9 1.887(4) .
Mo2 O3 1.898(6) .
Mo2 O3 1.898(6) 5_565
Mo2 O6 2.454(9) .
Mo2 O6 2.454(10) 8_565
P1 O5 1.52(2) 7_775
P1 O5 1.52(2) .
P1 O6 1.526(14) 9_655
P1 O6 1.526(14) 7_775
P1 O6 1.526(14) 2_765
P1 O6 1.526(14) 8_565
P1 O6 1.526(14) 3_675
P1 O6 1.526(14) .
O9 Mo2 1.887(4) 8_565
O1 Mo1 1.889(4) 2_765
O6 O5 1.759(19) 7_775
O6 O6 1.759(19) 9_655
O6 O6 1.759(19) 8_565
O6 Mo2 2.454(9) 9_655
O5 O6 1.759(19) 7_775
O5 O6 1.759(19) 9_655
O5 O6 1.759(19) 8_565
O5 Mo1 2.463(12) 8_565
O5 Mo1 2.463(12) 9_655
O5 Mo1 2.463(12) 7_775
Ag1 N1 2.26(2) .
Ag1 N2 2.762(19) 11_665
Ag2 N3 2.486(17) 6_656
Ag2 N3 2.486(17) .
N1 C1 1.32(3) .
N1 C2 1.34(3) .
N2 C1 1.32(3) .
N2 N3 1.36(2) .
N2 Ag1 2.762(19) 12_665
N3 C2 1.45(3) .
C1 H1 0.9300 .
C2 H2 0.9300 .
loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_4
O2 Mo1 O3 Mo2 -157.0(6) . .
O1 Mo1 O3 Mo2 19.4(14) . .
O1 Mo1 O3 Mo2 101.0(7) 3_675 .
O3 Mo1 O3 Mo2 -57.2(8) 10 .
O6 Mo1 O3 Mo2 6.3(6) . .
O5 Mo1 O3 Mo2 36.8(7) 7_775 .
O4 Mo2 O3 Mo1 157.6(6) . .
O9 Mo2 O3 Mo1 56.2(7) 9_655 .
O9 Mo2 O3 Mo1 -100.8(7) . .
O3 Mo2 O3 Mo1 -22.5(6) 5_565 .
O6 Mo2 O3 Mo1 -6.3(6) . .
O6 Mo2 O3 Mo1 -37.1(7) 8_565 .
O4 Mo2 O9 Mo2 -155.5(8) . 8_565
O9 Mo2 O9 Mo2 24.5(8) 9_655 8_565
O3 Mo2 O9 Mo2 103.9(9) . 8_565
O3 Mo2 O9 Mo2 -55.1(9) 5_565 8_565
O6 Mo2 O9 Mo2 39.1(10) . 8_565
O6 Mo2 O9 Mo2 8.2(8) 8_565 8_565
O2 Mo1 O1 Mo1 -154.5(9) . 2_765
O1 Mo1 O1 Mo1 -52.4(12) 3_675 2_765
O3 Mo1 O1 Mo1 29.0(17) . 2_765
O3 Mo1 O1 Mo1 105.4(10) 10 2_765
O6 Mo1 O1 Mo1 40.9(10) . 2_765
O5 Mo1 O1 Mo1 9.7(9) 7_775 2_765
O5 P1 O6 O5 180.000(3) . 7_775
O6 P1 O6 O5 119.8(6) 9_655 7_775
O6 P1 O6 O5 60.2(6) 2_765 7_775
O6 P1 O6 O5 -119.8(6) 8_565 7_775
O6 P1 O6 O5 -60.2(6) 3_675 7_775
O5 P1 O6 O6 -119.8(6) 7_775 9_655
O5 P1 O6 O6 60.2(6) . 9_655
O6 P1 O6 O6 -59.7(12) 2_765 9_655
O6 P1 O6 O6 120.3(12) 8_565 9_655
O6 P1 O6 O6 180.000(2) 3_675 9_655
O5 P1 O6 O6 119.8(6) 7_775 8_565
O5 P1 O6 O6 -60.2(6) . 8_565
O6 P1 O6 O6 -120.3(12) 9_655 8_565
O6 P1 O6 O6 180.000(0) 2_765 8_565
O6 P1 O6 O6 59.7(12) 3_675 8_565
O5 P1 O6 Mo2 -119.8(6) 7_775 9_655
O5 P1 O6 Mo2 60.2(6) . 9_655
O6 P1 O6 Mo2 -0.001(1) 9_655 9_655
O6 P1 O6 Mo2 -59.7(12) 2_765 9_655
O6 P1 O6 Mo2 120.3(12) 8_565 9_655
O6 P1 O6 Mo2 179.999(1) 3_675 9_655
O5 P1 O6 Mo2 119.8(6) 7_775 .
O5 P1 O6 Mo2 -60.2(6) . .
O6 P1 O6 Mo2 -120.3(12) 9_655 .
O6 P1 O6 Mo2 180.000(1) 2_765 .
O6 P1 O6 Mo2 0.000(0) 8_565 .
O6 P1 O6 Mo2 59.7(12) 3_675 .
O5 P1 O6 Mo1 0.000(1) 7_775 .
O5 P1 O6 Mo1 180.000(1) . .
O6 P1 O6 Mo1 119.8(6) 9_655 .
O6 P1 O6 Mo1 60.2(6) 2_765 .
O6 P1 O6 Mo1 -119.8(6) 8_565 .
O6 P1 O6 Mo1 -60.2(6) 3_675 .
O6 P1 O5 O6 -120.000(2) 9_655 7_775
O6 P1 O5 O6 -60.000(2) 2_765 7_775
O6 P1 O5 O6 120.000(2) 8_565 7_775
O6 P1 O5 O6 60.000(2) 3_675 7_775
O6 P1 O5 O6 180.000(3) . 7_775
O6 P1 O5 O6 120.000(3) 7_775 9_655
O6 P1 O5 O6 60.000(4) 2_765 9_655
O6 P1 O5 O6 -120.000(4) 8_565 9_655
O6 P1 O5 O6 180.000(4) 3_675 9_655
O6 P1 O5 O6 -60.000(3) . 9_655
O6 P1 O5 O6 120.000(2) 9_655 8_565
O6 P1 O5 O6 -120.000(3) 7_775 8_565
O6 P1 O5 O6 180.000(2) 2_765 8_565
O6 P1 O5 O6 -60.000(2) 3_675 8_565
O6 P1 O5 O6 60.000(3) . 8_565
O6 P1 O5 Mo1 120.000(2) 9_655 8_565
O6 P1 O5 Mo1 -120.000(0) 7_775 8_565
O6 P1 O5 Mo1 180.000(1) 2_765 8_565
O6 P1 O5 Mo1 0.000(1) 8_565 8_565
O6 P1 O5 Mo1 -60.000(2) 3_675 8_565
O6 P1 O5 Mo1 60.000(0) . 8_565
O6 P1 O5 Mo1 0.000(2) 9_655 9_655
O6 P1 O5 Mo1 120.000(3) 7_775 9_655
O6 P1 O5 Mo1 60.000(3) 2_765 9_655
O6 P1 O5 Mo1 -120.000(3) 8_565 9_655
O6 P1 O5 Mo1 180.000(2) 3_675 9_655
O6 P1 O5 Mo1 -60.000(4) . 9_655
O6 P1 O5 Mo1 -120.000(2) 9_655 7_775
O6 P1 O5 Mo1 0.000(0) 7_775 7_775
O6 P1 O5 Mo1 -60.000(1) 2_765 7_775
O6 P1 O5 Mo1 120.000(1) 8_565 7_775
O6 P1 O5 Mo1 60.000(2) 3_675 7_775
O6 P1 O5 Mo1 180.000(0) . 7_775
C1 N2 N3 C2 1(3) . .
Ag1 N2 N3 C2 174.9(15) 12_665 .
C1 N2 N3 Ag2 -171.2(14) . .
Ag1 N2 N3 Ag2 3(2) 12_665 .
C2 N1 C1 N2 -3(2) . .
Ag1 N1 C1 N2 -169(2) . .
N3 N2 C1 N1 1(2) . .
Ag1 N2 C1 N1 -172.5(18) 12_665 .
C1 N1 C2 N3 3(3) . .
Ag1 N1 C2 N3 170.9(15) . .
N2 N3 C2 N1 -2(3) . .
Ag2 N3 C2 N1 165.0(18) . .
